Firstorder reversal curve (FORC) diagrams for pseudosingledomain magnetites at high temperature


 Rhoda Ward
 1 years ago
 Views:
Transcription
1 Earth and Planetary Science Letters 203 (2002) 369^382 Firstorder reversal curve (FORC) diagrams for pseudosingledomain magnetites at high temperature Adrian R. Muxworthy,David J. Dunlop Geophysics, Physics Department, University of Toronto, Toronto, ON, Canada Received 17 May 2002; received in revised form 31 July 2002; accepted 31 July 2002 Abstract The recently developed firstorder reversal curve (FORC) technique for rapidly examining magnetic domain state has great potential for paleomagnetic and environmental magnetic investigations. However,there are still some gaps in the basic understanding of FORC diagrams,in particular the behavior of pseudosingledomain (PSD) grains and the contribution of magnetostatic interactions. In this paper we address some of these problems. We report the first FORC diagrams measurements on narrowly sized and wellcharacterized synthetic PSD through multidomain (MD) magnetite samples. The FORC diagrams evolve with grain size from singledomain (SD)like to MDlike through the PSD grain size range. Since each sample contains grains of essentially a single size,individual PSD grains evidently contain contributions from both SDlike and MDlike magnetic moments,in proportions that vary with grain size; the evolving FORC diagrams cannot be due to physical mixtures of SD and MD grains of widely different sizes. The FORC diagrams were all asymmetric. Small PSD samples have FORC diagrams with a distinctive closedcontour structure. The distributions of the larger MD grains display no peak,and lie closer to the interactionfield axis. To assess the effect of magnetostatic interactions,we measured FORC diagrams between room temperature and the Curie temperature. On heating the FORC distributions contract without changing shape until V500 C. Above this temperature the diagrams become more MDlike,and in addition become more symmetric. The temperature dependence of the interactionfield parameter is proportional to that of the saturation magnetization,in accordance with Ne el s interpretation of the Preisach diagram. The decrease in asymmetry with heating suggests that the origin of the asymmetry lies in magnetostatic interactions. The magnetic hysteresis parameters as a function of temperature were determined from the FORC curves. As the grain size decreased the normalized coercive force was found to decrease more rapidly with temperature. ß 2002 Elsevier Science B.V. All rights reserved. Keywords: magnetite; magnetic domains; coercivity; reversals 1. Introduction * Corresponding author. Present address: Department of Geology and Geophysics,University of Edinburgh,King s Buildings,West Mains Road,Edinburgh EH9 3JW,UK. Fax: address: (A.R. Muxworthy). The composition and grainsize distribution of magnetic minerals determine the overall magnetic properties of a rock or sediment and the stability of its natural remanent magnetization through geological time. With the increasing interest in using natural magnetic mineral assemblages in en X / 02 / $ ^ see front matter ß 2002 Elsevier Science B.V. All rights reserved. PII: S X(02)
2 370 A.R. Muxworthy, D.J. Dunlop / Earth and Planetary Science Letters 203 (2002) 369^382 vironmental and paleoclimatic studies,it is becoming essential to have magnetic methods that characterize both composition and grain size of the magnetic minerals. Conventional methods, calibrated using wellde ned synthetic samples, are unfortunately sometimes ambiguous in characterizing natural rocks and sediments [1]. The smallest magnetic grains,containing only a single domain (SD),have the strongest and most stable remanence. The iron oxide minerals,e.g. magnetite (Fe 3 O 4 ) and maghemite (QFe 2 O 3 ), dominate the magnetic properties of sediments and most continental rocks,both because of their common occurrence and their strong spontaneous magnetization. Grains above the SD/multidomain (MD) threshold size (70^100 nm; [2]) are often termed pseudosingledomain (PSD) because their remanence is also relatively strong and stable. PSD grains are usually volumetrically dominant in a typical rock or sediment. It is essential to have a reliable method or methods of determining the domain state in geological samples. In absolute paleointensity studies, SD grains produce the most reliable results and larger MD grains the least meaningful results, with PSD grains intermediate in their reliability [3]. Paleoclimatic information is often revealed by subtle changes in grainsize distribution,as revealed by domain state,while the same grainsize variations complicate the determination of relative paleo eld intensity from the same sediments [4]. One standard way of determining the domain state is measurement of magnetic hysteresis. Hysteresis parameters,such as coercive force H C, remanent coercive force H CR,saturation magnetization M S and the saturation remanence M RS, are often used for this purpose,either individually or in combination as in the plot of Day et al. [5]. However,the Day plot is nonunique: various combinations of mineral composition,grain size, internal stress and magnetostatic grain interactions can produce the same set of hysteresis parameters [6,7]. 2. The rstorder reversal curve (FORC) diagram Roberts et al. [1] and Pike et al. [8^10] have developed a new method of mineral and domain state discrimination using FORCs. Constructing a FORC diagram requires lengthy measurements and intricate mathematical analysis which have only recently become possible with fast and sensitive vibratingsample magnetometers (VSMs) and alternatinggradient magnetometers. The FORC diagram is constructed from a set of partial hysteresis curves (FORCs or rstorder return branches: [11,12]). Each FORC is measured by saturating the sample,decreasing the eld to a value H a,and reversing the eld sweep to the saturated state in a series of eld steps (H b ). This process is repeated for many values of H a. The magnetization M(H a,h b ) measured at each step generates the FORC distribution [1]: b ðh a ; H b Þr3D 2 MðH a ; H b Þ=DH a DH b ð1þ When the FORC distribution is plotted as a contour plot of b(h a,h b ),it is convenient to rotate axes by changing coordinates from {H a,h b } to {H C =(H b 3H a )/2, H U =(H b +H a )/2}. The FORC method originated in the phenomenological Preisach^Ne el theory of hysteresis. In the analogous Preisach [13] diagram (with a = H a s 0, b = H b 6 0),Ne el [14] showed that for interacting SD grains, H C corresponds to the coercive force H C of each SD loop in the absence of interactions and that H U is the local interaction eld. It follows that b(h a,h b ) is the product of two independent distributions,the coercivity distribution g(h C ) and the interaction eld distribution f(h U ). The Preisach and FORC distributions are equivalent in some situations,but in general the FORC diagram is less restrictive. For example,the FORC diagram does not assume a symmetric distribution. This symmetry restriction has been addressed in Preisach theory by the moving Preisach model,in which H U changes in proportion to the overall magnetization of the sample. This modi cation has been moderately successful (e.g. [15]),but introduces some ambiguity into the interpretation of measured Preisach diagrams. In general the philosophy of the FORC method is to reject any underlying modeldependent assumptions or approximations,e.g. as in the phenomenological Preisach model. Instead the FORC
3 A.R. Muxworthy, D.J. Dunlop / Earth and Planetary Science Letters 203 (2002) 369^ distribution is simply a wellde ned mathematical transformation of a suite of experimentally measured partial hysteresis curves [1]. Our study presents measurements of FORC distributions for PSD grains of magnetite at high temperature approaching the Curie temperature. FORC distributions for sized PSD magnetites have not been reported previously,although Preisach diagrams have been [15^19]. Another objective of the present study was to test whether or not pro les through the FORC distribution parallel to the H C and H U axes have the properties expected of distributions of coercivities g(h C ) and interaction elds f(h U ) as suggested by Ne el s interpretation of Preisach theory. Dunlop and West [16] and Dunlop et al. [19] determined Preisach diagrams using forward and reverse remanence measurements as a function of temperature. Their most striking nding was that the parameter H U usually interpreted as the interaction eld did not vary with temperature T as M S (T) as expected for magnetostatic interactions,but in fact as the coercive force H C (T). We carry out the same test on pro les of our FORC distributions and nd a temperature variation of f(h U ) that is compatible with M S (T). 3. Sample description Two sets of PSD and MD samples of di erent origin are studied in this paper. The rst set, W(0.3 Wm),W(1.7 Wm),W(7 Wm) and W(11 Wm),consists of commercial magnetites from Wright Industries produced six months before the experiments and stored in a desiccator. Grain sizes determined from scanning electron micrographs were all lognormally distributed. Xray di raction (XRD) spectra measured shortly after receiving the samples appeared to be those of pure magnetite,within experimental error. Six months later at the time the FORC measurements were made at the Institute for Rock Magnetism,Minnesota,USA,Mo«ssbauer spectra measured using a 57 Co source revealed oxidation parameters z ranging from for W(0.3 Wm) to for W(11 Wm). It is uncertain whether partial oxidation occurred during the six months of storage or whether the samples were initially nonstoichiometric. The stoichiometry was magnetically estimated from Curie and Verwey temperatures. A typical high eld thermomagnetic curve measured with a Princeton Measurements VSM is shown in Fig. 1. The Curie temperatures of 583 þ 1 C for the four samples are slightly higher than the 575^580 C of stoichiometric magnetite [20],again indicating a degree of nonstoichiometry. Verwey transitions determined from lowtemperature susceptibility measurements using a Lakeshore Cryotronics AC susceptometer were sharp in the larger grains, indicating stoichiometric magnetite,but broader in the smaller grains. The second set of samples,h(7.5 Wm),H(39 Wm) and H(76 Wm),was produced by hydrothermal recrystallization [21]. The magnetic properties of these samples have been described in detail by Muxworthy and McClelland [22] and Muxworthy Table 1 Grainsize distributions and roomtemperature hysteresis data for the studied samples Sample name Mean SD Mean AR W 0 H C W 0 H CR M RS /M S (Wm) (Wm) (mt) (mt) W(0.3Wm) W(1.7 Wm) W(7 Wm) W(11 Wm) H(7.5 Wm) ^ H(39 Wm) 39 9 ^ H(76 Wm) ^ The grainsize distributions were determined from scanning electron micrographs. The aspect ratio (AR) is the ratio of the long axis over the short axis. No aspect ratio was measured for the hydrothermally produced samples as they were nearly all symmetrical.
4 372 A.R. Muxworthy, D.J. Dunlop / Earth and Planetary Science Letters 203 (2002) 369^ Experimental methods Fig. 1. Hightemperature detail of a thermomagnetic curve for sample W(7 Wm). The Curie temperature is 584 C. This value is a little above the value often quoted for stoichiometric magnetite (575^580 C, [20]). The applied eld was 1 T. [23]. Mean grain sizes and standard deviations are summarized in Table 1. XRD and Mo«ssbauer spectra indicated pure magnetite and the samples had been stored for several years in nonoxidizing environments. However,to check for possible oxidation,warming curves for a saturation isothermal remanence induced at 35 K were measured using a Quantum Designs SQUID magnetometer. A sharp Verwey transition was observed,indicating stoichiometric magnetite and that little or no oxidation had occurred in these samples. Magnetic hysteresis parameters measured at room temperature for all seven samples using the VSM are summarized in Table 1 and shown with the mixing model of Dunlop [6] in the form of a Day plot in Fig. 2. The hydrothermally grown samples have very low values of H C and M RS /M S,close to those reported previously [22], indicating low dislocation densities in agreement with previous studies [24]. The Wright samples have higher H C and M RS /M S values than the hydrothermal samples of similar size,indicating a higher level of internal stress related either to the method of preparation or nonstoichiometry. H C and M RS /M S values decrease as grain size increases in agreement with other studies [5^7,25]. In Fig. 2,the smallest sample W(0.3 Wm) plots within the PSD region indicated by Dunlop [6]. The other Wright samples lie just above this PSD region,and the hydrothermal samples plot in the MD region. FORCs were measured using the VSM described above,for all seven samples at room temperature and at high temperature up to W600 C for the Wright samples. The samples were dispersed in hightemperature cement and heated in a helium atmosphere which,if anything,is slightly reducing (J. Marvin,personal communication, 2002). As there was a problem with the absolute temperature calibration for the VSM when measuring the FORCs,the VSM was initially manually calibrated for a range of temperatures using a second thermocouple. FORC diagrams were then measured for these set temperatures. Uncertainty in the absolute temperature at any step was þ 5 C. However,during the actual measurements at a particular step,the temperature did not vary by more than þ 1 C. The technique used for tting the FORC surface was identical to that outlined by Roberts et al. [1],where a full description is given. Brie y,to evaluate the FORC distribution b(h a,h b )(Eq. 1) at a point P,a local square grid of points is considered with P at the center. The number of points on the local grid depends on a smoothing Fig. 2. M RS /M S versus H CR /H C (Day plot) for the four Wright samples and the three hydrothermally grown magnetite samples. Also depicted are PSD and MD regions determined by Dunlop [6]. The hysteresis parameters were measured at room temperature.
5 A.R. Muxworthy, D.J. Dunlop / Earth and Planetary Science Letters 203 (2002) 369^ Fig. 3. Roomtemperature FORC diagrams for the four Wright samples. Scaling factors: (a) SF = 2,(b) SF = 3,(c) SF = 2 and (d) SF = 2. factor (SF) and is given by (2SF+1) 2. For example for SF = 3,the smoothing is performed across a7u7 array of data points. The magnetization at these points is then tted with a polynomial surface of the form: a 1 +a 2 H a +a 3 H 2 a +a 4H b + a 5 H 2 b +a 6H a H b,where the value 3a 6 represents b(h a,h b ) at P. Taking the second derivative in Eq. 1 magni es the noise that is inevitably present in the magnetization measurements. Therefore, FORC diagrams produced with SF = 1 contains greater noise. This can be reduced by increasing the size of SF; however,the cost of increasing SF is that ne scale features disappear. In addition,in calculating the FORC distribution,no points are determined in the region between the H U axis and 2USFUFS (FS = eld spacing during the FORC measurement) and it is necessary to make an extrapolation of the FORC surface onto the H U axis. Increasing SF increases the error in this extrapolation. The FORC distribution of an assemblage of noninteracting SD particles is narrowly con ned to the central horizontal axis [1,8]. Magnetostatic interactions between SD grains causes vertical spread of the contours about the peak,while thermal relaxation of ne SD particles shifts the FORC distribution to lower coercivities [8,9]. In contrast MD FORC distributions have no central peak,and the contours tend to spread broadly parallel to the H U = 0 axis [1,10]. 5. Roomtemperature results on PSD and MD magnetite Roomtemperature FORC diagrams are shown for the four Wright samples in Fig. 3,and for the three hydrothermally grown samples in Fig. 4. The FORC distributions change markedly with grain size. Samples W(0.3 Wm) and W(1.7 Wm) display distinct closedcontour peaks between 25 and 50 mt in the FORC distribution,while the peak of the FORC distribution lie near the origin for the larger samples. The crosssection of the FORC distribution along the H C axis is plotted in Fig. 5. According to the Preisach^Ne el theory, this plot is the coercivity distribution g(h C ). This distribution is seen to evolve continuously with grain size (Figs. 3^5). The hydrothermally grown samples (Fig. 4) display more MDlike FORC diagrams than the Wright samples (Fig. 3) for samples with similar grain sizes,e.g. W(7 Wm) and H(7.5 Wm). This re ects di erences in internal stress and dislocation densities. Pro les of the FORC distributions in the H U direction gradually become broader and atter with increasing grain size. The behavior of the larger grains is consistent with observations on MD grains [10]. This change re ects the di erences between PSD (grains containing only a few less mobile walls) and MD (grains containing many mobile walls). In addition all the FORC
6 374 A.R. Muxworthy, D.J. Dunlop / Earth and Planetary Science Letters 203 (2002) 369^382 Fig. 4. Roomtemperature FORC diagrams (SF = 5) for the three hydrothermally grown magnetite samples. Same scaling as Fig. 3. distributions display strong asymmetry,which in Preisach diagrams is normally associated with the asymmetry of the interaction eld during measurement [12,26]. According to Preisach^Ne el SD theory,the H U parameter is related to magnetostatic grain interactions. The theory for MD grains is less well developed,but it is clear that a system of domain walls will undergo a series of Barkhausen jumps in both increasing and decreasing elds,with an increment of magnetization at each jump. The hysteresis loop of one MD grain will resemble a linked sequence of SD loops and will generate a number of di erent points on a FORC distribution [26]. Domain walls in a particular grain are Fig. 5. Representative crosssections along the H C axis (H U = 0) of the roomtemperature FORC distributions shown in Figs. 3 and 4. According to the Preisach^Ne el model this is the coercivity distribution. The H(7.5 Wm) curve drops o quickly near H C =0. best treated as a magnetostatically coupled system [27]. Thus magnetostatic interaction among domains within a grain does not shift the overall hysteresis loop,but it does result in a distribution of points in the H U direction [10]. Importantly the interaction between domain walls,although di erent from interactions between SD grains,is also proportional to M S. 6. Hightemperature FORC diagrams of PSD samples FORC diagrams were measured for the four Wright samples at either nine or 10 set temperatures up to the Curie temperature (Figs. 6 and 7). For all samples,the FORC distributions contract with increasing temperature,and the FORC distribution in the H C direction shifts towards the H U axis (Figs. 6^8). In particular the contours which are closed at roomtemperature in samples W(0.3 Wm) and W(1.7 Wm) move toward the H U axis before nally joining the axis (Figs. 6 and 8). The shape of the FORC distributions changes with temperature. The FORC distribution of the smaller samples becomes more MDlike at high temperatures. On approaching the Curie temperature it was di cult to obtain accurate FORC diagrams,because the magnetic signature of the samples became weak. The hysteresis parameters H C, M RS and M S were directly obtained from the FORC measure
7 A.R. Muxworthy, D.J. Dunlop / Earth and Planetary Science Letters 203 (2002) 369^ Fig. 6. FORC diagrams (SF = 2) at four elevated temperatures for sample W(0.3 Wm). The scaling for parts a and b is di erent from that for c and d. ments. It must be realized that determining the hysteresis parameters from FORC measurements may give slightly di erent values to those determined from standard hysteresis measurements because of di erences in eld history [12]. H C and M RS /M S are plotted as a function of temperature in Fig. 9. On approaching the Curie temperature, H C goes almost to zero. H C displays similar hightemperature behavior to that reported previously [24,28]. The rate of decrease is almost constant except at very high temperatures,suggesting thermo uctuation e ects are not signi cant at most temperatures [28]. The reduced saturation remanence similarly decreases with temperature (Fig. 9b). For sample W(0.3 Wm), M RS /M S displays a sharper decrease at high temperatures than the other three Wright samples. The most likely cause of this is chemical alteration during heating. Mo«ssbauer spectroscopy suggests that W(0.3 Wm) was initially the least stoichiometric making it the most likely to be a ected by some sort of alteration on heating,i.e. inversion or reduction. Representative transverse FORC distribution pro les in the H U direction (nominally interaction eld spectra) are shown for sample W(1.7 Wm) in Fig. 10. To ascertain how the interaction eld H U is related to the spontaneous magnetization,we consider H i which is de ned here as the full width of the distribution at half the maximum height (FWHM). Normalized H i,i.e. H i (T)/ Fig. 7. FORC diagrams (SF = 3) at four elevated temperatures for sample W(7 Wm). The scaling for parts a and b is di erent from that for c and d.
8 376 A.R. Muxworthy, D.J. Dunlop / Earth and Planetary Science Letters 203 (2002) 369^382 Fig. 8. Crosssections along the H c axis (H u = 0) for the FORC distributions measured as a function of temperature for sample W(0.3 Wm) (Fig. 6). The temperature for each curve is given in Celsius. The FORC distribution is multiplied by the reduced magnetization,i.e. M S (T)/M S (T 0 ),where T 0 = 25 C. Fig. 10. Crosssections taken in the H U direction through the maximum of the FORC distributions measured for sample W(1.7 Wm) at various temperatures. The normalized FORC distribution is multiplied by the reduced magnetization. The temperature for each curve is given in Celsius. H i (25 C) is plotted versus M S (T)/M S (25 C) for all four Wright samples (Fig. 11). Generally,there is a linear relationship between normalized H i and M S,in agreement with Ne el s interpretation of Preisach theory. W(7 Wm) displays strongly linear behavior,w(1.7 Wm) appears to be rather noisy, whilst both W(0.3 Wm) and W(11 Wm) show similar behavior which is not quite linear. Dunlop et al. [19] made similar comparisons of H i (T) and M S (T) for their Preisach diagrams. They did not nd a linear relationship; instead H i (T) was more closely related to H C (T). The relationship between H i (T) and H C (T) was tested in this study,but it was not found to be linear. It is suggested that the general trend is linear and that H U re ects the level of magnetostatic interactions. Fig. 9. As a function of temperature,(a) the coercive force and (b) the reduced remanence (M RS /M S ) for all four Wright samples. Fig. 11. Normalized H i versus the reduced magnetization at di erent temperatures for samples (a) W(0.3 Wm),(b) W(1.7 Wm),(c) W(7 Wm) and (d) W(11 Wm). Linear trends have been tted to the data. H i is the FWHM value from crosssections like those depicted in Fig. 10.
9 A.R. Muxworthy, D.J. Dunlop / Earth and Planetary Science Letters 203 (2002) 369^ Fig. 12. Normalized coercive force versus temperature for the data plotted in Fig. 9a,compared with previously published experimental data and theoretical curves. The samples of Muxworthy [22],Heider et al. [24],Dunlop and Bina [28] and Dunlop [36] were grown synthetic magnetites with mean grain sizes of 7.5 Wm (sample H(7.5 Wm) in this paper),12 Wm,1^5 Wm and 0.22 Wm, respectively. The 10^15 Wm sample of Dankers and Sugiura [33] is shown. It was produced by annealing a crushed sample. The sample of Oº zdemir and Dunlop [37] was a 4 mm single crystal. The theoretical curves of Moskowitz [34] were determined using a onedimensional pinning model and are for a 10 Wm grain with six di erent pinning regimes; (1) positive dislocation dipole, d/w 0 = 1,(2) single dislocation,positive dislocation dipole d/w 0 = 0.1,or positive dislocation dipole bounding a stacking fault d/w 0 = 0.1,(3) negative dislocation dipole,d/w 0 = 1,(4) negative dislocation dipole,d/w 0 = 0.1,(5) planar defects with exchange pinning d/w 0 = 0.1,and (6) for planar defects with anisotropy pinning d/w 0 = 0.1,where the ratio d/w 0 is the reduced defect width. This dimensionless parameter sets the size of the defect and remains constant with temperature. Muxworthy and Williams [35] used a threedimensional stressfree micromagnetic model to determine H C for a 0.3 Wm cubic grain. To check for chemical alteration during FORC diagram measurement at high temperatures, repeat roomtemperature measurements were made. In all of the samples there was evidence for some degree of alteration. For W(0.3 Wm), which displayed the most alteration,after heating W 0 H C decreased to 25.7 mt and M S after heating was 72% of the initial M S. W(1.7 Wm) displayed the second highest degree of alteration; W 0 H C after heating increased slightly to 17.2 mt and after heating M S was 88% of the initial M S. 7. Discussion There is no rigorous theory for interpreting FORC diagrams for PSD and MD grains. Attempts have been made at modeling MD behavior using a onedimensional domain wall system [10]. However,this model does not include domain wall nucleation or magnetostatic domain interactions,both of which are important during hysteresis especially in small MD grains [29,30]. The interpretation of the results in this paper is therefore based on general principles.
10 378 A.R. Muxworthy, D.J. Dunlop / Earth and Planetary Science Letters 203 (2002) 369^382 The roomtemperature FORC measurements on the Wright magnetite samples show that there is a gradual change in the FORC distribution from SDlike (Fig. 3a,b) to MDlike (Fig. 3c,d). Samples with mean grain sizes between 1.7 Wm and 7 Wm need to be measured to quantify the grain size where the closedcontour structure disappears. The disappearance of the closedcontour structure could also be an indicator of the PSD MD grainsize transition. Samples W(7 Wm) (Fig. 3c) and H(7.5 Wm) (Fig. 4a) have similar grainsize distributions,yet their FORC diagrams are markedly di erent. Sample H(7.5 Wm) s FORC diagram displays a smaller peak at the origin and is more spread out along the H U axis,i.e. it is more MDlike. As the samples were prepared for FORC measurement using the same technique,the only possible causes for the di erences are di erent dislocation densities and/or di erences in stoichiometry. Roberts et al. ([1], Fig. 10) illustrated a similar progression from more SDlike to more MDlike FORC distributions for sediment samples whose representative points on a Day plot had a parallel progression from SDlike to MDlike along the PSD trend. The sediments had potentially broad grainsize distributions,conceivably so broad as to include truly SD and MD endmembers,and so it was uncertain whether their FORC diagrams were characteristic of single PSD sizes or blended the properties of a wide size distribution. Our results are unambiguous. Each of our samples contains grains of a distinct size,and the FORC distributions shown in Figs. 3 and 4 therefore characterize individual parts of the PSD and MD size spectrum. The combination of SDlike and MDlike features is thus a true PSD characteristic,implying contributions from both SDlike and MDlike magnetic moments in grains of a particular size,the proportions varying with grain size. On heating the Wright samples to near the Curie temperature (Figs. 6 and 7),the FORC distributions contract toward the origin,but do not change signi cantly in shape or appearance until V500 C. If the contraction is primarily related to the decrease in M S and H C,then this implies that the dominant domain structure does not change signi cantly with temperature. This is observed especially for the larger grains. The smaller grains with closed contours at lower temperatures become more MDlike on heating above 500 C, with the disappearance of the closedcontour structure. There are two possible causes of this change in FORC distribution. The domain structure may become more MDlike or,alternatively,the domain structure may become truly SD and then increasingly superparamagnetic,i.e. the change in FORC distribution is a SD thermal relaxation e ect [9]. The rst explanation appears to be more likely because recent highresolution micromagnetic calculations [31] suggest that the SD^PSD transition size increases with temperature but it is still signi cantly below 0.3 Wm at 565 C. This observed change in dominant domain structure may represent a possible mechanism for domain reorganization on cooling,essential for kinematic thermoremanence acquisition models [32]. According to Ne el s interpretation of Preisach diagrams, H U OM S. If it is provisionally assumed that FORC distributions can be interpreted using Preisach theory,this relationship was found to be true at a variety of temperatures. In contrast, Dunlop et al. [19] found using Preisach diagrams for SD and small PSD samples that H U OH C. Initially this seems surprising,but there are certain di erences in experimental method which must be considered. First,the method of experimentation was di erent; in this study b(h a,h b ) was found by measuring FORCs,whereas,Dunlop et al. [19] determined b(h a,h b ) from remanence measurements. Secondly,there was a large di erence in the resolution used in determining b(h a,h b ); Dunlop et al. [19] used only 144 points to determine their distribution,whereas in this study V points were used. In addition,it is also necessary to brie y consider the Preisach^Ne el model. For MD grains the theory for either FORC or Preisach diagrams is not well developed. Even in a simple MD model,the interactions come from both other grains and from other magnetic domains within the grain under consideration (i.e. internal demagnetizing eld). However,the MD Preisach model is more complicated than this and arguments have
11 A.R. Muxworthy, D.J. Dunlop / Earth and Planetary Science Letters 203 (2002) 369^ been made that H U should depend on both the microcoercive force distribution and the magnetostatic interaction energy [12,26],although this has not been rigorously tested. Assuming this to be true,if H U is controlled by both H C and M S, then depending on the relative degree of interaction,the e ect may be dominated by either H C or M S. In this study,to try to produce strong signals at high temperatures near the Curie temperature, high concentrations of magnetite powder were mixed with the cement powder,typically on the order of 10^20% by volume. SD and PSD grains mixed in these concentrations are known to show di erent magnetic behavior to dispersed samples [33]. Dunlop et al. [19] used typical concentrations of only 1% by volume. Another potentially important di erence between Dunlop et al. s samples and ours is the microcoercive force distribution and the resultant strength of domainwall pinning (W. Williams, personal communication,2002). Highly stressed magnetite grains like ours will tend to have their domain walls strongly pinned at the same dislocations at all temperatures. Thus the change in magnetostatic interaction due to changing M s during heating will be the major e ect and the FORC distribution in the H U direction will contract in proportion to M s. Lowstress hydrothermal magnetites like those used by Dunlop et al. [19] contain fewer and weaker pinning sites. During heating,the walls have more freedom of movement,jumping from one pin to another as dictated by H C (T). In this situation,the FORC and Preisach distributions in the H U direction are likely to contract more as H C (T) than as M S (T). All the roomtemperature FORC diagrams are asymmetrical (Figs. 3 and 4),although the asymmetry decreases with temperature (Figs. 6 and 7). The origin of the asymmetry in MD grains has not been discussed in previous FORC papers. In Preisach theory,the distribution is constrained to be symmetrical. However,experimental Preisach distributions are often found to be asymmetrical [15]. Much work has been done to try to understand the asymmetry of the Preisach distribution. The primary approach has been the moving Preisach model mentioned in the introduction, which accommodates changes in the interaction eld by a mean eld approach. The classical Preisach theory assumes a constant local interaction eld independent of M(H). In the moving model,the e ective eld H eff is the sum of the applied eld plus an interaction eld proportional to the overall magnetization M(H) in the applied eld H: H eff ¼ H þ Q MðHÞ ð2þ The e ectiveness of the moving Preisach model is best illustrated by considering the work of Hejda and Zelinka [15],who measured b(h a,h b ) using FORCs in an approach identical to that described by Roberts et al. [1],the only di erence being their interpretation of the data. Hejda and Zelinka [15] considered both a classical Preisach model and a moving Preisach model. The moving Preisach model was able to account for most of the asymmetry seen in the classical Preisach model interpretation. Similarly Pike et al. [8,9] showed theoretically using a movingpreisachtype model for SD particles that both magnetostatic interactions and thermal relaxation e ects can cause asymmetry in FORC distributions. The fact that thermal relaxation e ects would be expected to increase with temperature,while the asymmetry was observed to decrease (Figs. 6 and 7),suggests that the asymmetry in Preisach/FORC diagrams is directly or partially related to nonlocal magnetostatic interaction elds. The persistence of some asymmetry at high temperatures might be related to a noninteraction e ect. Measurements on natural rock samples containing magnetite and hematite have found that the Preisach/FORC distributions are often asymmetrical,indicating that interactions are important in geological samples,e.g. [1,9,15]. Fabian and von Dobeneck [26] suggested that for natural samples with low concentrations of magnetic minerals the classical Preisach model can be used. This may be suitable for samples containing SD or small PSD grains where interactions are due to other grains. However,where interaction e ects are due primarily to domain interactions or internal demagnetizing elds,then this assumption
12 380 A.R. Muxworthy, D.J. Dunlop / Earth and Planetary Science Letters 203 (2002) 369^382 fails. It has been found that individual MD grains produce asymmetric FORC distributions [10]. 8. Coercive force at high temperatures Even though the understanding of hysteresis behavior of magnetite as a function of temperature is important for MD rock magnetic theories, few measurements have been reported for wellcharacterized stoichiometric magnetite. The normalized coercive force as a function of temperature for samples W(0.3 Wm)^W(11 Wm) is compared in Fig. 12 with the onedimensional pinning model of Moskowitz [34] and the threedimensional micromagnetic hysteresis model of Muxworthy and Williams [35]. Moskowitz [34] examined the e ect of various dislocation structures on coercive force as a function of temperature. Muxworthy and Williams [35] determined H C for a dislocationfree 0.3 Wm grain. Also depicted in Fig. 12 are experimental results of Muxworthy [22],Heider et al. [24],Dunlop and Bina [28],Dankers and Sugiura [33],Dunlop [36] and Oº zdemir and Dunlop [37]. The model results of Moskowitz [34] are for a 10 Wm grain,implying that the model should only be directly compared with the results for W(7 Wm) and W(11 Wm). Moskowitz [34] showed that the microcoercive force is grain size dependent. There is a consistent grainsizedependent behavior for normalized H C versus temperature (Fig. 12). Data for W(0.3 Wm) falls near Moskowitz s model 3 curve,while W(1.7 Wm) lies slightly above this curve. Both W(7 Wm) and W(11 Wm) plot near the model 2 curve. At lower temperatures,normalized H C values for W(7 Wm) are higher than those of W(11 Wm),but at higher temperatures W(11 Wm) has higher normalized H C. Comparing the experimental results of this paper with those of six other studies,w(0.3 Wm) and W(1.7 Wm) display similar behavior to the grown sample of Dunlop and Bina [28]. Sample W(7 Wm) displays behavior close to that of the annealed crushed samples of Dankers and Sugiura [33]. W(11 Wm) shows similar but less pronounced behavior to that of the hydrothermal magnetite sample of Muxworthy [22],in that at higher temperatures ( s 400 C) the normalized H C decreases less rapidly with temperature in agreement with the model results of Muxworthy and Williams [35] for a 0.3 Wm grain. Why sample W(0.3 Wm) does not display this behavior is unclear. On comparison with the model results of Moskowitz [34], the dominant pinning mechanism apparently changes with grain size. W(0.3 Wm) and W(1.7 Wm) are consistent with a type 3 model,w(7 Wm) with a type 2 model and for W(11 Wm) the dominant pinning mechanism changes with temperature,i.e. a combination model [34] seems more appropriate. The 0.22 Wm sample of Dunlop [36] and the 4 mm sample of Oº zdemir and Dunlop [37] display remarkably similar behavior,initially following the model 2 line,then switching to the model 1 curve at higher temperatures. The samples in this study have normalized H C (T) less than these two samples. 9. Conclusions FORC diagrams have been measured as a function of temperature for a suite of sized PSD magnetite samples,and at room temperature for a set of hydrothermally grown PSD and MD magnetite samples. These measurements improve our basic understanding of this potentially important new technique,helping us to assess the contribution of interactions and the origin of the asymmetry, as well as classifying for the rst time the behavior of PSD grains. FORC diagrams gradually evolve from SDlike to MDlike through the PSD grainsize range. Small PSD grains have FORC diagrams with a distinctive closed peak structure. The FORC distributions of larger MD grains lie closer to and spread out along the H U axis. The disappearance of the closed peak structure between samples W(1.7 Wm) and W(7 Wm) may indicate a boundary between PSD and MD behavior. The fact that each of our samples contains grains of a discrete size leaves no doubt that these FORC distributions are individually characteristic of PSD or MD behavior. They do not blend the properties of a broad size distribution. The evolution of the PSD diagrams from SDlike to MDlike testi es
13 A.R. Muxworthy, D.J. Dunlop / Earth and Planetary Science Letters 203 (2002) 369^ to the changing proportions of SDlike and MDlike magnetic moments in PSD grains of di erent sizes. On heating,the PSD FORC distributions contract without changing shape until V500 C. Above this temperature,the FORC diagrams become more MDlike,with the closedcontour structures disappearing. The interaction eld was temperature dependent in proportion to M S (T), in accordance with Ne el s [14] interpretation of the Preisach diagram. Dunlop et al. [19] found H U (T)OH C (T). It is suggested the di erence between the two studies is due to di erent magnetite concentrations and/or di erences in internal stress. In this study,the concentrations were approximately 10 times higher than those of Dunlop et al. [19]. The FORC diagrams were asymmetrical at room temperature,gradually becoming more symmetric with temperature. The decrease in asymmetry with heating suggests that its origin lies in magnetostatic interactions (OM S (T)). This idea is supported by the direct comparison of classical and movingmodel Preisach diagrams made by Hejda and Zelinka [15]. The temperature dependence of normalized coercive force varied with grain size. Samples W(0.3 Wm)^W(7 Wm) displayed similar smooth,nearly linear temperature dependences,with normalized H C for W(0.3 Wm) 6 W(1.7 Wm) 6 W(7 Wm). The trend for W(11 Wm) was similar to the experimental results of Muxworthy [22] and model results of Muxworthy and Williams [35],i.e. normalized H C did not decrease smoothly across the entire temperature range. Such behavior of H C is potentially the origin of the demagnetization of partial thermoremanence on cooling [32]. Acknowledgements We would like to thank Chris Pike for his helpful comments and also for providing the FORC analysis software. In addition we thank Bruce Moskowitz for providing the raw data for the theoretical curves in Fig. 12. Wyn Williams and Andrew Roberts are thanked for their constructive reviews. The measurements were carried out at the Institute for Rock Magnetism,University of Minnesota,which is funded by the Keck Foundation and the University of Minnesota. We thank Mike Jackson,Jim Marvin and Peat SÖlheid for help with measurements.[rv] References [1] A.P. Roberts,C.R. Pike,K.L. Verosub,FORC diagrams: A new tool for characterizing the magnetic properties of natural samples,j. Geophys. Res. 105 (2000) 28461^ [2] W. Williams,T.M. Wright,Highresolution micromagnetic models of ne grains of magnetite,j. Geophys. Res. 103 (1998) 30537^ [3] S. Levi,The e ect of magnetite particle size on paleointensity determinations of the geomagnetic eld,phys. Earth Planet. Inter. 13 (1977) 245^259. [4] S.P. Lund,M. Schwartz,Environmental factors a ecting geomagnetic eld palaeointensity estimates from sediments,in: B.A. Maher,R. Thompson (Eds.),Quaternary Climates,Environments and Magnetism,Cambridge University Press,Cambridge,1999,pp. 323^351. [5] R. Day,M.D. Fuller,V.A. Schmidt,Hysteresis properties of titanomagnetites: Grain size and composition dependence,phys. Earth Planet. Inter. 13 (1977) 260^267. [6] D.J. Dunlop,Theory and application of the Day plot (M rs /M s versus H cr /H c ) 1. Theoretical curves and tests using titanomagnetite data,j. Geophys. Res. 107 (2002) /2001JB [7] D.J. Dunlop,Theory and application of the Day plot (M rs /M s versus H cr /H c ) 2. Application to data for rocks, sediments,and soils,j. Geophys. Res. 107 (2002) / 2001JB [8] C.R. Pike,A.P. Roberts,K.L. Verosub,Characterizing interactions in ne magnetic particle systems using rst order reversal curves,j. Appl. Phys. 85 (1999) 6660^6667. [9] C.R. Pike,A.P. Roberts,K.L. Verosub,FORC diagrams and thermal relaxation e ects in magnetic particles,geophys. J. Int. 145 (2001a) 721^730. [10] C.R. Pike,A.P. Roberts,M.J. Dekkers,K.L. Verosub,An investigation of multidomain hysteresis mechanisms using FORC diagrams,phys. Earth Planet. Inter. 126 (2001b) 11^25. [11] I.D. Mayergoyz,Mathematical models of hysteresis, IEEE Trans. Magn. 22 (1986) 603^608. [12] G. Bertotti,Hysteresis in Magnetism,Academic Press, London,1998,558 pp. [13] F. Preisach,Uº ber die magnetische Nachwirkung,Z. Phys. 94 (1935) 277^302. [14] L. Ne el,remarques sur la the orie des proprie te s magne tiques des substances dures,appl. Sci. Res. B4 (1954) 13^ 24. [15] P. Hejda,T. Zelinka,Modeling of hysteresis processes in
14 382 A.R. Muxworthy, D.J. Dunlop / Earth and Planetary Science Letters 203 (2002) 369^382 magnetic rock samples using the Preisach diagram,phys. Earth Planet. Inter. 63 (1990) 32^40. [16] D.J. Dunlop,G.F. West,An experimental evaluation of single domain theories,rev. Geophys. 7 (1969) 709^757. [17] V.A. Ivanov,I.A. Khaburzaniya,L.Ye. Sholpo,Use of Preisach diagram for diagnosis of single and multidomain grains in rock samples,izv. Earth Phys. 17 (1981) 36^43. [18] V.A. Ivanov,L.Ye. Sholpo,Quantitative criteria for single and multidomain states in ferromagnetic minerals in rocks,izv. Earth Phys. 18 (1982) 612^616. [19] D.J. Dunlop,M.F. WestcottLewis,M.E. Bailey,Preisach diagrams and anhysteresis: do they measure interactions?, Phys. Earth Planet. Inter. 65 (1990) 62^77. [20] D.J. Dunlop,Oº. Oº zdemir,rock Magnetism: Fundamentals and Frontiers,Cambridge University Press,New York,1997,573 pp. [21] F. Heider,L.T. Bryndzia,Hydrothermal growth of magnetite crystals (1 Wm to 1 mm),j. Cryst. Growth 84 (1987) 50^56. [22] A.R. Muxworthy,E. McClelland,The causes of lowtemperature demagnetization of remanence in multidomain magnetite,geophys. J. Int. 140 (2000) 132^146. [23] A.R. Muxworthy,Magnetic hysteresis and rotational hysteresis properties of hydrothermally grown multidomain magnetite,geophys. J. Int. 149 (2002) 805^814. [24] F. Heider,D.J. Dunlop,N. Sugiura,Magnetic properties of hydrothermally recrystallised magnetite crystals,science 236 (1987) 1287^1290. [25] H. Mauritsch,M. Becke,V. Kropa cek,t. Zelinka,P. Hejda,Comparison of the hysteresis characteristics of synthetic samples with di erent magnetite and haematite contents,phys. Earth Planet. Inter. 46 (1987) 93^99. [26] K. Fabian,T. von Dobeneck,Isothermal magnetization of samples with stable Preisach functions: a survey of hysteresis,remanence,and rock magnetic parameters, J. Geophys. Res. 102 (1997) 17659^ [27] T. Moon,R.T. Merrill,Magnetic screening in multidomain material,j. Geomagn. Geolectr. 38 (1986) 883^894. [28] D.J. Dunlop,M.M. Bina,The coercive force spectrum of magnetite at high temperatures: evidence for thermal activation below the blocking temperature,geophys J. R. Astron. Soc. 51 (1977) 121^147. [29] D. Virdee,The in uence of magnetostatic interactions on the magnetic properties of magnetite,ph.d. thesis,university of Edinburgh,1999. [30] A.J. Newell,R.T. Merrill,Nucleation and stability of ferromagnetic states,j. Geophys. Res. 105 (2000) 19377^ [31] A.R. Muxworthy,C. Carvallo,D.J. Dunlop,W. Williams,Highresolution micromagnetic models examining magnetic stability of magnetite at elevated temperatures, J. Geophys. Res.,submitted. [32] E. McClelland,N. Sugiura,A kinematic model of TRM acquisition in multidomain magnetite,phys. Earth Planet. Inter. 46 (1987) 9^23. [33] P. Dankers,N. Sugiura,The e ects of annealing and concentration on the hysteresis properties of magnetite around the PSDMD transition,earth Planet. Sci. Lett. 56 (1981) 422^428. [34] B.M. Moskowitz,Micromagnetic study of the in uence of crystal defects on coercivity in magnetite,j. Geophys. Res. 98 (1993) 18011^ [35] A.R. Muxworthy,W. Williams,Micromagnetic calculation of coercive force as a function of temperature in pseudosingle domain magnetite,geophys. Res. Lett. 26 (1999) 1065^1068. [36] D.J. Dunlop,Temperature dependence of hysteresis in 0.04^0.22 Wm magnetites and implications for domain structure,phys. Earth Planet. Inter. 46 (1987) 100^119. [37] Oº. Oº zdemir,d.j. Dunlop,E ect of crystal defects and internal stress on the domain structure and magnetic properties of magnetite,j. Geophys. Res. 102 (1997) 20211^20224.
FIRSTORDER REVERSAL CURVE (FORC) DIAGRAMS
FIRSTORDER REVERSAL CURVE (FORC) DIAGRAMS Adrian R. Muxworthy* and Andrew P. Roberts School of Ocean and Earth Science, National Oceanography Centre, European Way, University of Southampton, Southampton,
More informationPreisach Models and FORC Diagrams: A Critical Appraisal from a Physicist's Perspective
Preisach Models and FORC Diagrams: A Critical Appraisal from a Physicist's Perspective R M. Roshko Department of Physics and Astronomy University of Manitoba Winnipeg, Manitoba, Canada First Order Reversal
More informationHightemperature magnetic stability of small magnetite particles
JOURNAL OF GEOPHYSICAL RESEARCH, VOL. 108, NO. B5, 2281, doi:10.1029/2002jb002195, 2003 Hightemperature magnetic stability of small magnetite particles Adrian R. Muxworthy 1 and David J. Dunlop Geophysics,
More informationFirstorder reversal curve (FORC) diagrams of natural and cultured biogenic magnetic particles
Click Here for Full Article JOURNAL OF GEOPHYSICAL RESEARCH, VOL. 112,, doi:10.1029/2006jb004575, 2007 Firstorder reversal curve (FORC) diagrams of natural and cultured biogenic magnetic particles Amy
More informationEM4: Magnetic Hysteresis
CHALMERS UNIVERSITY OF TECHNOLOGY GÖTEBORG UNIVERSITY EM4: Magnetic Hysteresis Lab manual (version 1.001a) Students:... &... Date:... /... /... Laboration passed:... Supervisor:... Date:... /... /... Raluca
More informationThe interaction of Cu(100)Fe surfaces with oxygen studied with photoelectron spectroscopy. I
5 The interaction of Cu(100)Fe surfaces with oxygen studied with photoelectron spectroscopy. I Mg Kα excited photoemission. Abstract The oxidation of Cu(100)Fe surfaces was studied using XPS. Surfaces
More informationMagnetic susceptibility and its variations with temperature, measuring field and operating frequency Examples from various rock types
Magnetic susceptibility and its variations with temperature, measuring field and operating frequency Examples from various rock types Identification of magnetic minerals and phases Grain size assessment
More informationMagnetic Media Measurements with a VSM
Magnetic Media Measurements with a VSM B. C. Dodrill Lake Shore Cryotronics, Inc. 575 McCorkle Blvd Westerville, Ohio 43082 The last 50 years have seen the development of methods for the digital storage
More informationAjit Kumar Patra (Autor) Crystal structure, anisotropy and spin reorientation transition of highly coercive, epitaxial PrCo films
Ajit Kumar Patra (Autor) Crystal structure, anisotropy and spin reorientation transition of highly coercive, epitaxial PrCo films https://cuvillier.de/de/shop/publications/1306 Copyright: Cuvillier Verlag,
More informationShape and depth solutions form third moving average residual gravity anomalies using the window curves method
Kuwait J. Sci. Eng. 30 2) pp. 95108, 2003 Shape and depth solutions form third moving average residual gravity anomalies using the window curves method ELSAYED M. ABDELRAHMAN, TAREK M. ELARABY AND KHALID
More informationEXPERIMENTAL STUDY OF STRUCTURAL ZONE MODEL FOR COMPOSITE THIN FILMS IN MAGNETIC RECORDING MEDIA APPLICATION
EXPERIMENTAL STUDY OF STRUCTURAL ZONE MODEL FOR COMPOSITE THIN FILMS IN MAGNETIC RECORDING MEDIA APPLICATION Hua Yuan and David E. Laughlin Department of Materials Science and Engineering, Carnegie Mellon
More informationPermanent Magnet Materials
Measurements with a VSM Permanent Magnet Materials B. C. Dodrill B. J. Kelley Lake Shore Cryotronics, Inc. 575 McCorkle Blvd. Westerville, OH, 43082 Please address correspondence to bdodrill@lakeshore.com
More informationIron Powder Cores for Switchmode Power Supply Inductors. by: Jim Cox
HOME APPLICATION NOTES Iron Powder Cores for Switchmode Power Supply Inductors by: Jim Cox Purpose: The purpose of this application note is to cover the properties of iron powder as a magnetic core material
More informationMagnetic Data Storage and Nanoparticles Ernie Chang
Magnetic Data Storage and Nanoparticles Ernie Chang Introduction Magnetic storage, specifically in hard drives has advanced significantly since the first disk drive built in 1956 [1]. Interestingly enough,
More informationKOLEKTOR MAGNET TECHNOLOGY
ZIT S KOERZIT S Sintered AlNiCo Koerzit is the KOLEKTOR MAGNET TECHNOLOGY GmbH tradename for sintered permanent magnets based on AlNi and AlNiCo alloys. Koerzit magnets are made by powder metallurgy. KOLEKTOR
More informationTHE EFFECT OF THE HDDR PROCESS ON THE PRODUCTION OF PrFeCoBNb SINTERED MAGNETS
THE EFFECT OF THE HDDR PROCESS ON THE PRODUCTION OF PrFeCoBNb SINTERED MAGNETS E. A. Ferreira, J. C. S. Casini, E. A. Périgo, R. N. Faria, H. Takiishi Av. Prof. Lineu Prestes, 2242  CEP 05508000,
More informationEFFECT OF PARTICLE SIZE DISTRIBUTION ON THE MICROSTRUCTURE AND MAGNETIC PROPERTIES OF SINTERED NdFeB MAGNETS
Effect Rev. Adv. of particle Mater. Sci. size 28 distribution (2011) 185189 on the microstructure and magnetic properties of sintered... 185 EFFECT OF PARTICLE SIZE DISTRIBUTION ON THE MICROSTRUCTURE
More informationModern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras
Modern Construction Materials Prof. Ravindra Gettu Department of Civil Engineering Indian Institute of Technology, Madras Module  2 Lecture  2 Part 2 of 2 Review of Atomic Bonding II We will continue
More informationChapter 8. Low energy ion scattering study of Fe 4 N on Cu(100)
Low energy ion scattering study of 4 on Cu(1) Chapter 8. Low energy ion scattering study of 4 on Cu(1) 8.1. Introduction For a better understanding of the reconstructed 4 surfaces one would like to know
More informationIN current film media, the increase in areal density has
IEEE TRANSACTIONS ON MAGNETICS, VOL. 44, NO. 1, JANUARY 2008 193 A New Read Channel Model for Patterned Media Storage Seyhan Karakulak, Paul H. Siegel, Fellow, IEEE, Jack K. Wolf, Life Fellow, IEEE, and
More informationInternational Year of Light 2015 TechTalks BREGENZ: Mehmet Arik WellBeing in Office Applications Light Measurement & Quality Parameters
www.ledprofessional.com ISSN 1993890X Trends & Technologies for Future Lighting Solutions ReviewJan/Feb 2015 Issue LpR 47 International Year of Light 2015 TechTalks BREGENZ: Mehmet Arik WellBeing in
More information4 Thermomechanical Analysis (TMA)
172 4 Thermomechanical Analysis 4 Thermomechanical Analysis (TMA) 4.1 Principles of TMA 4.1.1 Introduction A dilatometer is used to determine the linear thermal expansion of a solid as a function of temperature.
More informationNew Approach to Analysis of the Switching Current Data in Ferroelectric Thin Films
Ferroelectrics, 291: 27 35, 2003 Copyright c Taylor & Francis Inc. ISSN: 00150193 print / 15635112 online DOI: 10.1080/00150190390222510 New Approach to Analysis of the Switching Current Data in Ferroelectric
More informationAnomalous Hall Effect Magnetometry A Method for Studying Magnetic Processes of Thin Magnetic Films
Anomalous Hall Effect Magnetometry A Method for Studying Magnetic Processes of Thin Magnetic Films J. R. Lindemuth a, B. C. Dodrill a and N. C. Oldham b a Lake Shore Cryotronics, Inc. 575 McCorkle Blvd,
More informationIncorporating Internal Gradient and Restricted Diffusion Effects in Nuclear Magnetic Resonance Log Interpretation
The OpenAccess Journal for the Basic Principles of Diffusion Theory, Experiment and Application Incorporating Internal Gradient and Restricted Diffusion Effects in Nuclear Magnetic Resonance Log Interpretation
More informationSixstate, threelevel, sixfold ferromagnetic wire system
Sixstate, threelevel, sixfold ferromagnetic wire system T. Blachowicz 1a and A. Ehrmann 2 1 Institute of Physics, Silesian University of Technology, 44100 Gliwice, Poland 2 Faculty of Textile and Clothing
More informationk u (t) = k b + k s t
Chapter 2 Stripe domains in thin films 2.1 Films with perpendicular anisotropy In the first part of this chapter, we discuss the magnetization of films with perpendicular uniaxial anisotropy. The easy
More informationInsertion Devices Lecture 4 Permanent Magnet Undulators. Jim Clarke ASTeC Daresbury Laboratory
Insertion Devices Lecture 4 Permanent Magnet Undulators Jim Clarke ASTeC Daresbury Laboratory Introduction to Lecture 4 So far we have discussed at length what the properties of SR are, when it is generated,
More informationLecture Notes: Basic Concepts in Option Pricing  The Black and Scholes Model
Brunel University Msc., EC5504, Financial Engineering Prof Menelaos Karanasos Lecture Notes: Basic Concepts in Option Pricing  The Black and Scholes Model Recall that the price of an option is equal to
More informationAlgebra 1 Course Information
Course Information Course Description: Students will study patterns, relations, and functions, and focus on the use of mathematical models to understand and analyze quantitative relationships. Through
More information2. Permanent Magnet (De) Magnetization 2.1 Methodology
Permanent Magnet (De) Magnetization and Soft Iron Hysteresis Effects: A comparison of FE analysis techniques A.M. Michaelides, J. Simkin, P. Kirby and C.P. Riley Cobham Technical Services Vector Fields
More informationDirect Observation of Magnetic Gradient in Co/Pd PressureGraded Media
Direct Observation of Magnetic Gradient in Co/ PressureGraded Media B. J. Kirby 1,a), S. M. Watson 1, J. E. Davies 2, G. T. Zimanyi 3, Kai Liu 3, R. D. Shull 2, and J. A. Borchers 1 1 Center for Neutron
More informationAP Physics 1 and 2 Lab Investigations
AP Physics 1 and 2 Lab Investigations Student Guide to Data Analysis New York, NY. College Board, Advanced Placement, Advanced Placement Program, AP, AP Central, and the acorn logo are registered trademarks
More informationA direct comparison of the properties of CRM and VRM in the lowtemperature oxidation of magnetite
Geophys. J. lnt. (1991) 105, 407418 A direct comparison of the properties of CRM and VRM in the lowtemperature oxidation of magnetite A. K. Gapeev,'S. K. Gribov,' D. J. Dunlop,2 0. 0zdemir2 and V. P. Shcherbakov'
More informationOur development of economic theory has two main parts, consumers and producers. We will start with the consumers.
Lecture 1: Budget Constraints c 2008 Je rey A. Miron Outline 1. Introduction 2. Two Goods are Often Enough 3. Properties of the Budget Set 4. How the Budget Line Changes 5. The Numeraire 6. Taxes, Subsidies,
More informationXRay Study of Soft and Hard Magnetic Thin Films
Copyright (C) JCPDSInternational Centre for Diffraction Data 1999 13 XRay Study of Soft and Hard Magnetic Thin Films PoWen Wang, 390 Reed St., Stormedia, Inc., Santa Clara CA. 95050 Abstract : This
More informationData Mining Algorithm for Rock Magnetic Data Analysis
Data Mining Algorithm for Rock Magnetic Data Analysis WANWU GUO School of Computer and Information Science Edith Cowan University 2 Bradford Street, Mount Lawley, WA 6050, AUSTRALIA Abstract The correlation
More informationMarine broadband seismic: Is the earth response helping the resolution revolution? N. Woodburn*, A. Hardwick, and R. Herring, TGS
Marine broadband seismic: Is the earth response helping the resolution revolution? N. Woodburn*, A. Hardwick, and R. Herring, TGS Summary Broadband seismic aims to provide a greater richness of both (a),
More informationInterpreting Data in Normal Distributions
Interpreting Data in Normal Distributions This curve is kind of a big deal. It shows the distribution of a set of test scores, the results of rolling a die a million times, the heights of people on Earth,
More informationSimultaneous data fitting in ARXPS
NOTE Please find the following more updated document Resolving overlapping peaks in ARXPS data: The effect of noise and fitting method. J. MuñozFlores, A. HerreraGomez, J. Electron Spectrosc. Relat.
More informationThe accurate calibration of all detectors is crucial for the subsequent data
Chapter 4 Calibration The accurate calibration of all detectors is crucial for the subsequent data analysis. The stability of the gain and offset for energy and time calibration of all detectors involved
More informationIterative calculation of the heat transfer coefficient
Iterative calculation of the heat transfer coefficient D.Roncati Progettazione Ottica Roncati, via Panfilio, 17 44121 Ferrara Aim The plate temperature of a cooling heat sink is an important parameter
More informationEtudes in situ et ex situ de multicouches C/FePt
Etudes in situ et ex situ de multicouches C/FePt : influence de la température sur la structure et les propriétés s magnétiques D. Babonneau, G. Abadias, F. Pailloux Laboratoire de Physique des Matériaux
More informationAbsolute and Relative Gas Concentration: Understanding Oxygen in Air. Bruce Bugbee and Mark Blonquist
Absolute and Relative Gas Concentration: Understanding Oxygen in Air Bruce Bugbee and Mark Blonquist Absolute and Relative Gas Concentration Gas concentration is described in two ways, absolute and relative
More informationMicrocontrollerbased experiments for a control systems course in electrical engineering technology
Microcontrollerbased experiments for a control systems course in electrical engineering technology Albert LozanoNieto Penn State University, WilkesBarre Campus, Lehman, PA, USA Email: AXL17@psu.edu
More informationGuidance for Industry
Guidance for Industry Q2B Validation of Analytical Procedures: Methodology November 1996 ICH Guidance for Industry Q2B Validation of Analytical Procedures: Methodology Additional copies are available from:
More information15.062 Data Mining: Algorithms and Applications Matrix Math Review
.6 Data Mining: Algorithms and Applications Matrix Math Review The purpose of this document is to give a brief review of selected linear algebra concepts that will be useful for the course and to develop
More informationChapter 4. Magnetic Materials and Circuits
Chapter 4 Magnetic Materials and Circuits Objectives List six characteristics of magnetic field. Understand the righthand rule for current and magnetic fluxes. Define magnetic flux, flux density, magnetomotive
More informationLecture Notes  Sediment Transport The Sediment Problem. 1. The Difference Between τ c and τ r. 2. The Different Applications of Critical Shear Stress
Lecture Notes  Sediment Transport The Sediment Problem At the end of the first lecture, we noted that our steep, nonlinear transport model depended on τ*, which is the ratio of the bed shear stress τ
More informationNUCLEAR MAGNETIC RESONANCE. Advanced Laboratory, Physics 407, University of Wisconsin Madison, Wisconsin 53706
(revised 4/21/03) NUCLEAR MAGNETIC RESONANCE Advanced Laboratory, Physics 407, University of Wisconsin Madison, Wisconsin 53706 Abstract This experiment studies the Nuclear Magnetic Resonance of protons
More informationAn analysis of price impact function in orderdriven markets
Available online at www.sciencedirect.com Physica A 324 (2003) 146 151 www.elsevier.com/locate/physa An analysis of price impact function in orderdriven markets G. Iori a;, M.G. Daniels b, J.D. Farmer
More informationStudies on Pore Systems in Catalysts
JOURNAL OF CATALYSIS 4, 319323 (1965) Studies on Pore Systems in Catalysts V. The t Method B. C. LIPPENS* AND J. H. DE BOER From the Department of Chemical Technology, Technological University of Delft,
More informationHigh Resolution Spatial Electroluminescence Imaging of Photovoltaic Modules
High Resolution Spatial Electroluminescence Imaging of Photovoltaic Modules Abstract J.L. Crozier, E.E. van Dyk, F.J. Vorster Nelson Mandela Metropolitan University Electroluminescence (EL) is a useful
More informationApplication of sensitivity analysis in investment project evaluation under uncertainty and risk
International Journal of Project Management Vol. 17, No. 4, pp. 217±222, 1999 # 1999 Elsevier Science Ltd and IPMA. All rights reserved Printed in Great Britain 02637863/99 $  see front matter PII: S02637863(98)000350
More informationBoltzmann Distribution Law
Boltzmann Distribution Law The motion of molecules is extremely chaotic Any individual molecule is colliding with others at an enormous rate Typically at a rate of a billion times per second We introduce
More informationG 3. AN ELECTRONIC JOURNAL OF THE EARTH SCIENCES Published by AGU and the Geochemical Society
Geosystems G 3 AN ELECRONIC JOURNAL OF HE EARH SCIENCES Published by AGU and the Geochemical Society Article Volume 5, Number 2 26 February 24 Q2H7, doi:.29/23gc63 ISSN: 525227 oward an optimal geomagnetic
More informationELECTRIC FIELD LINES AND EQUIPOTENTIAL SURFACES
ELECTRIC FIELD LINES AND EQUIPOTENTIAL SURFACES The purpose of this lab session is to experimentally investigate the relation between electric field lines of force and equipotential surfaces in two dimensions.
More informationHuman resource allocation in a multiproject R&D environment
International Journal of Project Management Vol. 17, No. 3, pp. 181±188, 1999 # 1998 Elsevier Science Ltd and IPMA. All rights reserved Printed in Great Britain 02637863/98 $19.00 + 0.00 PII: S02637863(98)00026X
More informationDESCRIPTIVE STATISTICS. The purpose of statistics is to condense raw data to make it easier to answer specific questions; test hypotheses.
DESCRIPTIVE STATISTICS The purpose of statistics is to condense raw data to make it easier to answer specific questions; test hypotheses. DESCRIPTIVE VS. INFERENTIAL STATISTICS Descriptive To organize,
More informationSimulation of Residual Stresses in an Induction Hardened Roll
2.6.4 Simulation of Residual Stresses in an Induction Hardened Roll Ludwig Hellenthal, Clemens Groth Walzen Irle GmbH, NetphenDeuz, Germany CADFEM GmbH, Burgdorf/Hannover, Germany Summary A heat treatment
More informationWe can display an object on a monitor screen in three different computermodel forms: Wireframe model Surface Model Solid model
CHAPTER 4 CURVES 4.1 Introduction In order to understand the significance of curves, we should look into the types of model representations that are used in geometric modeling. Curves play a very significant
More informationRecent development in piezoelectric materials used for actuators and sensors applications
Recent development in piezoelectric materials used for actuators and sensors applications Dragan Damjanovic, Ceramics Laboratory, Materials Institute Swiss Federal Institute of Technology  EPFL Lausanne
More informationSTANDARD CLEANING AND CALIBRATION PROCEDURE FOR TGA50(H) AND TGA51(H)
STANDARD CLEANING AND CALIBRATION PROCEDURE FOR TGA50(H) AND TGA51(H) by Joseph F. Greenbeck, Jr. And Courtney W. Taylor INTRODUCTION The following procedure is to be used for the maintenance and calibration
More informationFeatures of the formation of hydrogen bonds in solutions of polysaccharides during their use in various industrial processes. V.Mank a, O.
Features of the formation of hydrogen bonds in solutions of polysaccharides during their use in various industrial processes. V.Mank a, O. Melnyk b a National University of life and environmental sciences
More informationHEAT TRANSFER ANALYSIS IN A 3D SQUARE CHANNEL LAMINAR FLOW WITH USING BAFFLES 1 Vikram Bishnoi
HEAT TRANSFER ANALYSIS IN A 3D SQUARE CHANNEL LAMINAR FLOW WITH USING BAFFLES 1 Vikram Bishnoi 2 Rajesh Dudi 1 Scholar and 2 Assistant Professor,Department of Mechanical Engineering, OITM, Hisar (Haryana)
More informationNew Method for Optimum Design of Pyramidal Horn Antennas
66 New Method for Optimum Design of Pyramidal Horn Antennas Leandro de Paula Santos Pereira, Marco Antonio Brasil Terada Antenna Group, Electrical Engineering Dept., University of Brasilia  DF terada@unb.br
More informationChapter Outline: Phase Transformations in Metals
Chapter Outline: Phase Transformations in Metals Heat Treatment (time and temperature) Microstructure Mechanical Properties Kinetics of phase transformations Multiphase Transformations Phase transformations
More informationGlancing XRD and XRF for the Study of Texture Development in SmCo Based Films Sputtered Onto Silicon Substrates
161 162 Glancing XRD and XRF for the Study of Texture Development in SmCo Based Films Sputtered Onto Silicon Substrates F. J. Cadieu*, I. Vander, Y. Rong, and R. W. Zuneska Physics Department Queens College
More informationMAGNETIC PHASE AND DOMAIN EVOLUTION OF
PhD thesis booklet MAGNETIC PHASE AND DOMAIN EVOLUTION OF ANTIFERROMAGNETICALLY COUPLED MULTILAYERS Márton Major Eötvös Loránd University Faculty of Science Doctorate School of Physics Material Science
More informationImplied Volatility for FixedResets
Implied Volatility for FixedResets In this essay I explain the calculation of Implied Volatility for FixedResets, in accordance with a spreadsheet I have developed which is publicly available at http://www.prefblog.com/xls/impliedvolatility.xls.
More informationPlate waves in phononic crystals slabs
Acoustics 8 Paris Plate waves in phononic crystals slabs J.J. Chen and B. Bonello CNRS and Paris VI University, INSP  14 rue de Lourmel, 7515 Paris, France chen99nju@gmail.com 41 Acoustics 8 Paris We
More informationGas Dynamics Prof. T. M. Muruganandam Department of Aerospace Engineering Indian Institute of Technology, Madras. Module No  12 Lecture No  25
(Refer Slide Time: 00:22) Gas Dynamics Prof. T. M. Muruganandam Department of Aerospace Engineering Indian Institute of Technology, Madras Module No  12 Lecture No  25 PrandtlMeyer Function, Numerical
More informationThe Metropolis Algorithm
The Metropolis Algorithm Statistical Systems and Simulated Annealing Physics 170 When studying systems with a great many particles, it becomes clear that the number of possible configurations becomes exceedingly
More informationCharacterization of Polyketone Copolymer by High Speed DSC
application Note Thermal Analysis Authors Wim M. Groenewoud Eerste Hervendreef 32 5232 JK S Hertogenbosh The Netherlands Nik Boer PerkinElmer, Groningen The Netherlands Phil Robinson Thermal Analysis Consultant
More informationELECTRON SPIN RESONANCE Last Revised: July 2007
QUESTION TO BE INVESTIGATED ELECTRON SPIN RESONANCE Last Revised: July 2007 How can we measure the Landé g factor for the free electron in DPPH as predicted by quantum mechanics? INTRODUCTION Electron
More informationC;Ri.N. (o3s8: Université Louis Pasteur de Strasbourg. Institut National de Physique Nucléaire et de Physique des Particules t...
(o3s8: C;Ri.N CWMB 7»fi CO i\ ANGULAR ASSÏMBTRIBS IN A SHIELDED ^ PAIR LINE CO CJ H.FANMarri, C.A. GMCIA CANAL «nd H. VUCETICH o \. CHRKE DE «CH.1RCHES KKXEAIRES UHIVERSITB LOUIS PASTEUR STRASBOURG
More informationHOW ACCURATE ARE THOSE THERMOCOUPLES?
HOW ACCURATE ARE THOSE THERMOCOUPLES? Deggary N. Priest Priest & Associates Consulting, LLC INTRODUCTION Inevitably, during any QC Audit of the Laboratory s calibration procedures, the question of thermocouple
More informationFederal Institute for Materials Research and Testing
Federal Institute for Materials Research and Testing CERTIFIED REFERENCE MATERIAL FOR THE GAS ADSORPTION BAMPM101 Material: SiO 2 with specific surface area (BET) of 0.177 0.004 m² g 1 Mean of means
More informationIronCarbon Phase Diagram (a review) see Callister Chapter 9
IronCarbon Phase Diagram (a review) see Callister Chapter 9 University of Tennessee, Dept. of Materials Science and Engineering 1 The Iron Iron Carbide (Fe Fe 3 C) Phase Diagram In their simplest form,
More informationThe successful integration of 3D seismic into the mining process: Practical examples from Bowen Basin underground coal mines
Geophysics 165 Troy Peters The successful integration of 3D seismic into the mining process: Practical examples from Bowen Basin underground coal mines This paper discusses how mine staff from a number
More informationThere are certain things that we have to take into account before and after we take an FID (or the spectrum, the FID is not that useful after all).
Data acquisition There are certain things that we have to take into account before and after we take an FID (or the spectrum, the FID is not that useful after all). Some deal with the detection system.
More informationNuclear Magnetic Resonance
Nuclear Magnetic Resonance NMR is probably the most useful and powerful technique for identifying and characterizing organic compounds. Felix Bloch and Edward Mills Purcell were awarded the 1952 Nobel
More informationApplication of Nuclear Magnetic Resonance in Petroleum Exploration
Application of Nuclear Magnetic Resonance in Petroleum Exploration Introduction Darko Tufekcic, consultant email: darkotufekcic@hotmail.com Electromagnetic resonance method (GEOEMR) is emerging as the
More informationRadiative effects of clouds, ice sheet and sea ice in the Antarctic
Snow and fee Covers: Interactions with the Atmosphere and Ecosystems (Proceedings of Yokohama Symposia J2 and J5, July 1993). IAHS Publ. no. 223, 1994. 29 Radiative effects of clouds, ice sheet and sea
More informationES250: Electrical Science. HW7: Energy Storage Elements
ES250: Electrical Science HW7: Energy Storage Elements Introduction This chapter introduces two more circuit elements, the capacitor and the inductor whose elements laws involve integration or differentiation;
More informationLaboratory scale electrical resistivity measurements to monitor the heat propagation within porous media for low enthalpy geothermal applications
32 CONVEGNO NAZIONALE 1921 Novembre 2013 TRIESTE Laboratory scale electrical resistivity measurements to monitor the heat propagation within porous media for low enthalpy geothermal applications N. Giordano
More informationDetermining Measurement Uncertainty for Dimensional Measurements
Determining Measurement Uncertainty for Dimensional Measurements The purpose of any measurement activity is to determine or quantify the size, location or amount of an object, substance or physical parameter
More informationOxidation behaviour of Ti 3 SiC 2 based ceramic at 900±1300 C in air
Corrosion Science 43 2001) 1095±1109 www.elsevier.com/locate/corsci Oxidation behaviour of Ti 3 SiC 2 based ceramic at 900±1300 C in air Zhimei Sun a, Yanchun Zhou a, *, Meishuan Li b a Department of
More informationElectrochemical Kinetics ( Ref. :Bard and Faulkner, Oldham and Myland, Liebhafsky and Cairns) R f = k f * C A (2) R b = k b * C B (3)
Electrochemical Kinetics ( Ref. :Bard and Faulkner, Oldham and Myland, Liebhafsky and Cairns) 1. Background Consider the reaction given below: A B (1) If k f and k b are the rate constants of the forward
More informationA METHOD OF CALIBRATING HELMHOLTZ COILS FOR THE MEASUREMENT OF PERMANENT MAGNETS
A METHOD OF CALIBRATING HELMHOLTZ COILS FOR THE MEASUREMENT OF PERMANENT MAGNETS Joseph J. Stupak Jr, Oersted Technology Tualatin, Oregon (reprinted from IMCSD 24th Annual Proceedings 1995) ABSTRACT The
More informationXray photoelectron. Ba 0.5 Sr 0.5 Co 0.8 Fe 0.2 O 3 δ and La 0.6 Sr 0.4 Co 0.2 Fe 0.8 O 3 δ before and after thermal treatment and permeation test
study on Ba 0.5 Sr 0.5 Co 0.8 Fe 0.2 O 3 δ and La 0.6 Sr 0.4 Co 0.2 Fe 0.8 O 3 δ before and after thermal treatment and permeation test Patrizia Rosa 1 1 Dipartimenti di Fisica Università degli Studi di
More informationSENSITIVITY ANALYSIS AND INFERENCE. Lecture 12
This work is licensed under a Creative Commons AttributionNonCommercialShareAlike License. Your use of this material constitutes acceptance of that license and the conditions of use of materials on this
More informationA Complete Gradient Clustering Algorithm for Features Analysis of Xray Images
A Complete Gradient Clustering Algorithm for Features Analysis of Xray Images Małgorzata Charytanowicz, Jerzy Niewczas, Piotr A. Kowalski, Piotr Kulczycki, Szymon Łukasik, and Sławomir Żak Abstract Methods
More informationCOMPACT CORIOLIS MASS FLOW METER/CONTROLLER FOR LOW FLOWS
COMPACT CORIOLIS MASS FLOW METER/CONTROLLER FOR LOW FLOWS W. Jouwsma Bronkhorst CoriTech B.V. Nijverheidsstraat , 71 AK Ruurlo, The Netherlands Phone: +31 573 59; Fax: +31 9375; Internet: www.bronkhorstcoritech.com
More informationDETERMINATION OF THE HEAT STORAGE CAPACITY OF PCM AND PCMOBJECTS AS A FUNCTION OF TEMPERATURE. E. Günther, S. Hiebler, H. Mehling
DETERMINATION OF THE HEAT STORAGE CAPACITY OF PCM AND PCMOBJECTS AS A FUNCTION OF TEMPERATURE E. Günther, S. Hiebler, H. Mehling Bavarian Center for Applied Energy Research (ZAE Bayern) WaltherMeißnerStr.
More informationAN INVESTIGATION INTO THE USEFULNESS OF THE ISOCS MATHEMATICAL EFFICIENCY CALIBRATION FOR LARGE RECTANGULAR 3 x5 x16 NAI DETECTORS
AN INVESTIGATION INTO THE USEFULNESS OF THE ISOCS MATHEMATICAL EFFICIENCY CALIBRATION FOR LARGE RECTANGULAR 3 x5 x16 NAI DETECTORS Frazier L. Bronson CHP Canberra Industries, Inc. 800 Research Parkway,
More informationPhysics 9e/Cutnell. correlated to the. College Board AP Physics 1 Course Objectives
Physics 9e/Cutnell correlated to the College Board AP Physics 1 Course Objectives Big Idea 1: Objects and systems have properties such as mass and charge. Systems may have internal structure. Enduring
More informationHamed Aber 1 : Islamic Azad University, Science and Research branch, Tehran, Iran. Mir Sattar Meshin chi asl 2 :
Present a Proper Pattern for Choose Best Electrode Array Based on Geological Structure Investigating in Geoelectrical Tomography, in order to Get the Highest Resolution Image of the Subsurface Hamed Aber
More informationExploratory data analysis (Chapter 2) Fall 2011
Exploratory data analysis (Chapter 2) Fall 2011 Data Examples Example 1: Survey Data 1 Data collected from a Stat 371 class in Fall 2005 2 They answered questions about their: gender, major, year in school,
More informationBARE PCB INSPECTION BY MEAN OF ECT TECHNIQUE WITH SPINVALVE GMR SENSOR
BARE PCB INSPECTION BY MEAN OF ECT TECHNIQUE WITH SPINVALVE GMR SENSOR K. Chomsuwan 1, S. Yamada 1, M. Iwahara 1, H. Wakiwaka 2, T. Taniguchi 3, and S. Shoji 4 1 Kanazawa University, Kanazawa, Japan;
More information